Ag2O | AlF3 | As2O3 | As4O6 | Au2O3 | BaF2 | BeO | CaF2 | CdO | CeO2 | CrO3 | Cs2O | Cu2O | CuCO3 | Dy2O3 | Er2O3 | Eu2O3 | F | Fr2O | Free SiO2 | Ga2O3 | GdO3 | GeO2 | HfO2 | HgO | Ho2O3 | In2O3 | IrO2 | KF | KNaO | La2O3 | Lu2O3 | Mn2O3 | MnO2 | MoO3 | N2O5 | NaF | Nb2O5 | Nd2O3 | NiO | OsO2 | P2O5 | Pa2O5 | PbF2 | PdO | PmO3 | PO4 | Pr2O3 | PrO2 | PtO2 | RaO | Rb2O | Re2O7 | RhO3 | RuO2 | Sb2O3 | Sb2O5 | Sc2O3 | Se | SeO2 | Sm2O3 | Ta2O5 | Tb2O3 | Tc2O7 | ThO2 | Tl2O | Tm2O3 | U3O8 | UO2 | WO3 | Y2O3 | Yb2O3 | ZrO
•The secret to cool bodies and glazes is a lot of testing.
•The secret to know what to test is material and chemistry knowledge.
•The secret to learning from testing is documentation.
•The place to test, do the chemistry and document is an account at https://insight-live.com
•The place to get the knowledge is https://digitalfire.com
Sign-up at https://insight-live.com today.
|COLE - Co-efficient of Linear Expansion||0.148|
|GSPT - Frit Softening Point||2910C (From The Oxide Handbook We also have a figure of 2572?)|
CaO is not found pure in nature but rather is contained in various abundant minerals (i.e. calcite, aragonite, limestone, marble) but vary greatly in their purity (impurities usually include magnesia, iron, alumina, silica, sulfur). Of these iron and sulfur are most troublesome (i.e. where clarity is important in glass). Lime minerals vary in the degree of crystallization and cohesion of the crystalline mass and the homogeneity of the matrix.
-Together with SrO, BaO, and MgO it is considered one of the Alkaline Earth group of oxides. It has a cubic crystal structure.
-Quicklime is pure calcia, but it reacts with water to produce calcium hydroxide or slaked lime. Calcium oxide, on the other hand, is an extremely stable compound.
-Calcia alone resists melting even at very high temperatures (around an incredible 2600C), but when soda and potash are added, it becomes very active in both oxidation and reduction. At higher temperatures, CaO contributed by wollastonite is more readily fusible than that contributed by whiting (calcium carbonate). This synergy between CaO and other fluxes and differences in the mechanism of its fluxing action generates some disagreement among experts regarding the nature of CaO (like MgO, it is not a 'stand-alone' flux).
-Calcium oxide is the principle flux in medium and high temperature glazes, beginning its action (within the glaze) around 1100C. It must be used with care in high-fire bodies because its active fluxing action can produce a body that is too volatile (melting if slightly overfired).
-Calcia usually hardens a glaze and makes it more scratch and acid resistant. This is especially so in alkaline and lead glazes. However the increased hardness does not necessarily mean greater tensile strength. Its thermal expansion is intermediate.
-CaO is not effective below cone 4 as a flux in glazes but in small amounts (less than 10%) it can dissolve in earthenware glaze melts especially with lead, soda, potash) to add hardness and resistance to leaching. In non-lead mixes it can also help reduce crazing. In larger amounts, it encourages the growth of crystals which can give decorative effects to glossy glazes and produce matteness (i.e. 30%).
-High CaO glazes tend to devitrify (crystallize). This occurs either because of the high melt fluidity imparted by CaO at higher temperatures or because of the readiness with which CaO forms crystals. Fastfire glazes can contain more CaO because the quick cooling does not give the crystallization a chance to occur.
-Calcia is a moderate flux in the cone 5-6 range, but a very active one at cone 10.
-High calcia glazes tend to have good (although sometimes unexpected) color responses. For example, in oxidation iron glazes calcia likes to form yellow crystalline compounds with the Fe2O3 producing a 'lime matte'. Without the calcia, glossy brown glazes are the norm.
The term 'lime' encompasses several different minerals and manufactured products.
-The term 'Whiting' traditionally refers to calcium carbonate produced by the grinding of chalk from the cliffs of England, Belgium and France. However this title also refers to any ground calcium carbonate material (i.e. those processed from marble and calcite ores).
-Ground limestone and calcined limestone (burned lime) are used in the glass industry. Float and container glass have 10% CaO.
-Dolomite (magnesium carbonate) is a mineral which supplies some magnesia in addition to its CaO complement. It is preferred in many situations because it more readily fluxes and the magnesia imparts desirable properties.
-Wollastonite is a calcium silicate which is more expensive than other sources of calcium, but is used bodies, glaze, porcelains, enamels and frits for its many superior properties.
Glaze Color - Yellow
In oxidation, iron glazes calcia likes to form yellow crystalline compounds with the Fe2O3 producing a 'lime matte' even in an otherwise fluid glaze.
Glaze Color - Glossy Brown, Black
Calcia likes to form yellow crystalline compounds with Fe2O3 producing a 'lime matte', especially in fluid glazes. Thus iron glossy brown or black glazes should be low in CaO.
Glaze Matteness - Lime Crystal Matte
High molar amounts of calcia combined with adequate silica and preferably lower alumina will form a calcium silicate crystal matte (lime matte). The presence of zinc will increase the size of crystals.
Glaze Variegation - General
CaO can mottle glaze surfaces at high temperatures if significant amounts are present, it is a very strong flux and can contribute to phase separation.
In the glaze on the left (90% Ravenscrag Slip and 10% iron oxide) the iron is saturating the melt crystallizing out during cooling. GR10-K1, on the right, is the same glaze but with 5% added calcium carbonate. This addition is enough to keep most of the iron in solution through cooling, so it contributes to the super-gloss deep tenmoku effect instead of precipitating out.
These are two cone 6 matte glazes (shown side by side in an account at Insight-live). G1214Z is high calcium and a high silica:alumina ratio (you can find more about it by googling 1214Z). It crystallizes during cooling to make the matte effect and the degree of matteness is adjustable by trimming the silica content (but notice how much it runs). The G2928C has high MgO and it produces the classic silky matte by micro-wrinkling the surface, its matteness is adjustable by trimming the calcined kaolin. CaO is a standard oxide that is in almost all glazes, 0.4 is not high for it. But you would never normally see more than 0.3 of MgO in a cone 6 glaze (if you do it will likely be unstable). The G2928C also has 5% tin, if that was not there it would be darker than the other one because Ravenscrag Slip has a little iron. This was made by recalculating the Moore's Matte recipe to use as much Ravenscrag Slip as possible yet keep the overall chemistry the same. This glaze actually has texture like a dolomite matte at cone 10R, it is great. And it has wonderful application properties. And it does not craze, on Plainsman M370 (it even survived and 300F to ice water plunge without cracking). This looks like it could be a great liner glaze.
2, 5, 10, 15% calcium carbonate added to Ravenscrag Slip on a buff stoneware fired at cone 10R. It gets progressively glossier toward 15%, crazing starts at 10% (test by Kat Valenzuela). Adding a flux only reduces the SiO2 and Al2O3, this pushes the thermal expansion upwards. 5% is actually sufficient. An alternative would be to use wollastonite, it supplies SiO2 also.
These glaze cones are fired at cone 6 and have the same recipe: 20 Frit 3134, 21 EP Kaolin, 27 calcium carbonate, 32 silica. The difference: The one on the left uses dolomite instead of calcium carbonate. Notice how the MgO from the dolomite completely mattes the surface whereas the CaO from the calcium carbonate produces a brilliant gloss.
Two glazes, same chemistry, different materials. The glaze on the left is sourcing CaO from wollastonite, the one on the right from calcium carbonate. Thus the oxide chemistry of the two is the same but the recipe of materials sourcing that chemistry is different. The difference in the melt flow you see here is an expression of how choosing different mineral sources to source an oxide can produce melting patterns that go outside what the chemistry suggests. The difference here is not extreme, but it can be much more. Glaze chemistry is relative, not absolute. It works best when you are changing material amounts, not material types. When you do introduce a very different mineral then you have a different system which has its own relative chemistry.
This high boron cone 04 glaze is generating calcium-borate crystals during cool down (called boron-blue). This is a common problem and a reason to control the boron levels in transparent glazes; use just enough to melt it well. If a more melt fluidity is needed, decrease the percentage of CaO. For opaque glazes, this effect can actually enable the use of less opacifier.
Stull chart showing the SiO2-Al2O3-(0.7CaO+0.3KNaO) system
Phase diagram and stull chart showing the SiO2-Al2O3-(0.7CaO+0.3KNaO) system. Courtesy of Matthew Katz, Alfred University
Left: a cone 6 matte glaze (G2934 with no colorant). Middle: 5% Mason 6006 chrome-tin red stain added. Right: 5% Mason 6021 encapsulated red stain added. Why is there absolutely no color in the center glaze? This host recipe does not have the needed chemistry to develop the #6006 chrome-tin color (it lacks sufficient CaO and has alot of MgO). Yet this same matte glaze intensifies the #6021 encapsulated stain at only 5% (using 20% or more encapsulated stain is to develop the color is not unusual).
We are looking at two pairs of samples, they demonstrate why knowing about glaze chemistry can be so important. Both pairs are the same glazes: G2934 cone 6 matte and G2916F cone 6 glossy. The left pair has 5% maroon stain added, the right pair 5% purple stain. The red and purple develop correctly in the glossy but not the matte. Why? The Mason Colorworks reference guide has the same precaution for both stains: the host glaze must be zincless and have 6.7-8.4% CaO (this is a little unclear, it is actually expressing a minimum, the more the CaO the better). The left-most samples of each pair here have 11% CaO, the right-most have 9%. So there is enough CaO. The problem is MgO (it is the mechanism of the matteness in the left two), it impedes the development of both colors. When you talk to tech support at any stain company, as I did with Mason on this, they need to know the chemistry of your glaze to help, not the recipe.
All common traditional ceramic base glazes are made from only a dozen elements (plus oxygen). Materials decompose when glazes melt, sourcing these elements in oxide form. The kiln builds the glaze from these, it does not care what material sources what oxide (assuming, of course, that all materials do melt or dissolve completely into the melt to release those oxides). Each of these oxides contributes specific properties to the glass. So, you can look at a formula and make a good prediction of the properties of the fired glaze. And know what specific oxide to increase or decrease to move a property in a given direction (e.g. melting behavior, hardness, durability, thermal expansion, color, gloss, crystallization). And know about how they interact (affecting each other). This is powerful. And it is simpler than looking at glazes as recipes of hundreds of different materials (each sources multiple oxides so adjusting it affects multiple properties).
Out Bound Links
Carbonate of Lime, Whiting, Aragonite, Calcite, CaCO3
Lime Spar, Lime Feldspar, Ca-Feldspar
Calcium Magnesium Carbonate, Raw Limestone
Burnt Lime, Dead-burned lime
The term 'limit formula' historically has typically referred to efforts to establish absolute ranges for mixtures of oxides that melt well at an intended temperature and are not in sufficient excess to cause defects. These formulas typically show ranges for each oxide commonly used in a specific gla...
In Bound Links
Glaze chemistry models fired glazes as constructed of oxides decomposed from the materials in the recipe. Fired properties of glazes (like melting temperature, thermal expansion, surface character, even color) are a product of the oxide makeup (the chemistry). Oxides are grouped in various ways to s...
In a glaze melt, oxides do not act alone, they interact. For example, while one material might not melt well by itself, when combined with others the mix as a whole can melt at a significantly lower temperature than any of the ingredients in the mix. Cornwall stone is an example, by itself it does n...
On the theoretical glaze chemistry level, a flux is an oxide that lowers the melting or softening temperature of a mix of materials. Fluxes are interactors (they often melt poorly on their own but react strongly with high melting materials where Al2O3/SiO2 predominate). There are less than ten commo...
An oxide is a combination of oxygen and another element. There are only about ten common oxides that we need to learn about (most glazes have half that number). CaO (a flux), SiO2 (a glass former) and Al2O3 (an intermediate) are examples of oxides. CaO (calcium oxide or calcia), for example, is cont...